VIEWS: 21 PAGES: 44 POSTED ON: 11/19/2012
MECHANICAL PROPERTIES OF MATERIALS Manufacturing Processes, 1311 Dr Simin Nasseri Southern Polytechnic State University MECHANICAL PROPERTIES OF MATERIALS 1. Stress-Strain Relationships (Slide 4) 2. Tensile Test (Slide 7) 3. Compression Test (Slide 36) Manufacturing Processes Prof Simin Nasseri Mechanical Properties in Design and Manufacturing Mechanical properties determine a material’s behavior when subjected to mechanical stresses Properties include elastic modulus, ductility, hardness, and various measures of strength Dilemma: mechanical properties desirable to the designer, such as high strength, usually make manufacturing more difficult The manufacturing engineer should appreciate the design viewpoint And the designer should be aware of the manufacturing viewpoint Manufacturing Processes Prof Simin Nasseri Strain- Stress Relationship Stress-Strain Relationships Three types of static stresses to which materials can be subjected: 1. Tensile - tend to stretch the material 2. Compressive - tend to squeeze it 3. Shear - tend to cause adjacent portions of material to slide against each other Stress-strain curve - basic relationship that describes mechanical properties for all three types Manufacturing Processes Prof Simin Nasseri Various Tests Manufacturing Processes Prof Simin Nasseri Tensile Test Most common test for studying stress-strain relationship, especially metals In the test, a force pulls the material, elongating it and reducing its diameter Figure 3.1 Tensile test: (a) tensile force applied in (1) and (2) resulting elongation of material Manufacturing Processes Prof Simin Nasseri Tensile Test Specimen ASTM (American Society for Testing and Materials) specifies preparation of test specimen Figure 3.1 Tensile test: (b) typical test specimen Manufacturing Processes Prof Simin Nasseri Tensile Test Setup Manufacturing Processes Prof Simin Nasseri Tensile Test Sequence Figure 3.2 Typical progress of a tensile test: If pieces are put back together as (1) (2) uniform (3) continued (4) necking (5) in (6), final length beginning elongation and elongation, begins, load fracture can be measured of test, no reduction of maximum load begins to load cross-sectional reached decrease Manufacturing Processes area Prof Simin Nasseri Tensile Test Manufacturing Processes Prof Simin Nasseri Different types of stress-strain graphs Engineering important in design Stress-strain curves True important in manufacturing Manufacturing Processes Prof Simin Nasseri Engineering Stress Defined as force divided by original area: F e Ao where e = engineering stress (MPa) or Pa or psi, F = applied force (N) or lb, and Ao = original area of test specimen (mm2 or m2 or in2) (Remember: N/ m2 = Pa, N/ mm2 = MPa, lb/ in2 = psi, klb/ in2 = kips/ in2) Manufacturing Processes Prof Simin Nasseri Engineering Strain Defined at any point in the test as L Lo e Lo where e = engineering strain (it has no unit); L = length at any point during elongation; and Lo = original gage length Manufacturing Processes Prof Simin Nasseri Typical Engineering Stress-Strain Plot Figure 3.3 Typical engineering stress-strain plot in a tensile test of a metal. Manufacturing Processes Prof Simin Nasseri Two Regions of Stress-Strain Curve The two regions indicate two distinct forms of behavior: 1. Elastic region – prior to yielding of the material 2. Plastic region – after yielding of the material Manufacturing Processes Prof Simin Nasseri Elastic Region in Stress-Strain Curve Relationship between stress and strain is linear Material returns to its original length when stress is removed Hooke's Law: e = E e where E = modulus of elasticity, e = stress, e=strain E is a measure of the inherent stiffness of a material Its value differs for different materials Manufacturing Processes Prof Simin Nasseri Yield Point in Stress-Strain Curve As stress increases, a point in the linear relationship is finally reached when the material begins to yield Yield point Y can be identified by the change in slope at the upper end of the linear region Y = a strength property Other names for yield point = yield strength, yield stress, and elastic limit Manufacturing Processes Prof Simin Nasseri Plastic Region in Stress-Strain Curve Yield point marks the beginning of plastic deformation The stress-strain relationship is no longer guided by Hooke's Law (non-linear relationship) As load is increased beyond Y, elongation proceeds at a much faster rate than before, causing the slope of the curve to change dramatically Manufacturing Processes Prof Simin Nasseri Tensile Strength in Stress-Strain Curve Elongation is accompanied by a uniform reduction in cross-sectional area, consistent with maintaining constant volume Finally, the applied load F reaches a maximum value, and engineering stress at this point is called the tensile strength TS (or ultimate tensile strength) Fmax TS = Ao Manufacturing Processes Prof Simin Nasseri Ductility in Tensile Test Ability of a material to plastically strain without fracture Ductility measure = elongation EL Lf Lo EL Lo where EL = elongation (expresses as a percent); Lf = specimen length at fracture; and Lo = original specimen length Lf is measured as the distance between gage marks after two pieces of specimen are put back together Manufacturing Processes Prof Simin Nasseri Area reduction defined as A0 Af AR A0 expressed as a percent, where: Af = area of the cross section at the point of fracture, mm2 or in2 A0 = original area Therefore, ductility is measured by elongation (EL) or area reduction (AR). Manufacturing Processes Prof Simin Nasseri Lets compare! Which material has the highest modulus of elasticity? Which material has the highest tensile strength? Which material has the highest elongational rate? Manufacturing Processes Prof Simin Nasseri Lets compare! LOW - - - - - - - - - - - - - - - - - - - - - - - - > HIGH Modulus of elasticity (measure of stiffness): Polyethylene (0.03x106 psi), Nylon, Lead (3x106 psi), Magnesium, AL & Glass, Copper, Cast Iron (20x106 psi), Iron & Steel (30x106 psi), Alumina (50x106 psi), Tungsten, Diamond (150x106 psi) stress has lower E strain For a given force, the one with lower E, deforms more in comparison with the one with higher E (which is stiffer). Manufacturing Processes Prof Simin Nasseri Lets compare! LOW - - - - - - - - - - - - - - - - - - - - - - - - > HIGH Tensile Strength: AL (10,000psi), Copper, Cast Iron (40,000psi), Mg, Low C Steel, High C Steel(90,000psi), Stainless steel (95,000psi), Ti alloy Elongation: Metals: Cast Iron (0.6%), Mg, high C steel (10%), Ti, low C steel (30%), Nickel, Stainless steel (55%). Ceramics: 0% Polymers: thermosetting polymer (1%), Thermoplastic polymer (100%) Manufacturing Processes Prof Simin Nasseri True Stress Stress value obtained by dividing the applied load by the instantaneous area F A In elastic region they are almost the same where = true stress; F = force; and A = actual (instantaneous) area resisting the load Manufacturing Processes Prof Simin Nasseri True Strain or Hencky strain Provides a more realistic assessment of "instantaneous" elongation per unit length L dL L d ln L ln L0 ln Lo L Lo L ln Lo Manufacturing Processes Prof Simin Nasseri True Stress-Strain Curve Figure 3.4 - True stress-strain curve for the previous engineering stress-strain plot in Figure 3.3. Manufacturing Processes Prof Simin Nasseri Strain Hardening in Stress-Strain Curve Note that true stress increases continuously in the plastic region until necking In the engineering stress-strain curve, the significance of this was lost because stress was based on an incorrect area value It means that the metal is becoming stronger as strain increases This is the property called strain hardening Manufacturing Processes Prof Simin Nasseri True stress versus Engineering Stress True strain can be related to the corresponding engineering strain ln 1 e by: True stress and engineering stress can be related by the t e 1 e expression: True stress versus true strain in plastic region: K is the strength coefficient and is t K n Flow curve in MPa. n is the strain hardening exponent. Manufacturing Processes Prof Simin Nasseri Flow Curve True stress-strain curve a straight line in a log-log plot: ln ln K K n n ln ln K ln n ln ln K n ln this is similar to: if =1, then Y b nX K Figure 3.5 True stress-strain curve plotted on log-log scale. Manufacturing Processes Prof Simin Nasseri Lets compare! Engineering Stress & strain True Stress & strain F F e Ao Elastic region e = E e t E A L Lo L dL L e ln Lo t e 1 e L L o Lo TS = Fmax ln 1 e TS = Fmax Ao A Plastic region t K n Manufacturing Processes Prof Simin Nasseri Lets compare! Toughness: area under strain-stress graph (combination of ductility and strength) Manufacturing Processes Prof Simin Nasseri Categories of Stress-Strain Relationship Perfectly elastic Elastic and perfectly plastic Elastic and strain hardening Manufacturing Processes Prof Simin Nasseri Perfectly Elastic Behavior is defined completely by modulus of elasticity E Fractures rather than yielding to plastic flow Brittle materials: ceramics, many cast irons, and thermosetting polymers Figure 3.6 Categories of stress-strain relationship: (a) perfectly elastic. Manufacturing Processes Prof Simin Nasseri Elastic and Perfectly Plastic Stiffness defined by E K Once Y reached, deforms plastically at same stress level Flow curve: K = Y, n = 0 Metals behave like this when heated to sufficiently high temperatures (above Figure 3.6 Categories of recrystallization) stress-strain relationship: One example is Lead (b) elastic and perfectly plastic. Manufacturing Processes Prof Simin Nasseri Elastic and Strain Hardening Hooke's Law in elastic K n region, yields at Y Flow curve: K > Y, n > 0 Most ductile metals behave this way when cold worked Figure 3.6 Categories of stress-strain relationship: (c) elastic and strain hardening. Manufacturing Processes Prof Simin Nasseri Compression test Compression Test Applies a load that squeezes the ends of a cylindrical specimen between two platens Figure 3.7 Compression test: (a) compression force applied to test piece in (1) and (2) resulting change in height. Manufacturing Processes Prof Simin Nasseri Compression Test Setup Manufacturing Processes Prof Simin Nasseri Engineering Stress in Compression As the specimen is compressed, its height is reduced and cross-sectional area is increased e = - F Ao where Ao = original area of the specimen Manufacturing Processes Prof Simin Nasseri Engineering Strain in Compression Engineering strain is defined h ho e ho Since height is reduced during compression, value of e is negative (the negative sign is usually ignored when expressing compression strain) Manufacturing Processes Prof Simin Nasseri Stress-Strain Curve in Compression Shape of plastic region is different from tensile test because cross section increases Calculated value of engineering stress is higher In comparison to the true stress Figure 3.8 Typical engineering stress-strain curve for a compression test. Manufacturing Processes Prof Simin Nasseri Tensile Test vs. Compression Test Although differences exist between engineering stress-strain curves in tension and compression, the true stress-strain relationships are nearly identical Since tensile test results are more common, flow curve values (K and n) from tensile test data can be applied to compression operations When using tensile K and n data for compression, ignore necking, which is a phenomenon peculiar to straining induced by tensile stresses Barreling and edge fracture happen Manufacturing Processes Prof Simin Nasseri
"MECHANICAL PROPERTIES OF MATERIALS - Southern "